Large-Displacement Structural Durability Analyses of ... Large-displacement elastic and...
Embed Size (px)
Transcript of Large-Displacement Structural Durability Analyses of ... Large-displacement elastic and...
NASA Technical Memorandum 106521
Large-Displacement Structural Durability Analyses of Simple Bend Specimen Emulating Rocket Nozzle Liners
Vinod K. Arya University of Toledo Toledo, Ohio
Gary R. Halford Lewis Research Center Cleveland, Ohio
National Aeronautics and
LARGE-DISPLACEMENT STRUCTURAL DURABILITY ANALYSES OF SIMPLE BEND SPECIMEN EMULATING
ROCKET NOZZLE LINERS
Vinod K. Arya* University of Toledo Toledo, Ohio 43606
Gary R. Halford National Aeronautics and Space Administration
Lewis Research Center Cleveland, Ohio 44135
Large-displacement elastic and elastic-plastic, finite-element stress-strain analyses of an oxygen- free high-conductivity (OFHC) copper plate specimen were performed using an updated Lagrangian for- mulation. The plate specimen is intended for low-cost experiments that emulate the most important thermomechanical loading and failure modes of a more complex rocket nozzle. The plate, which is loaded in bending at 593 °C, contains a centrally located and internally pressurized channel. The cyclic crack initiation lives were estimated using the results from the analyses and isothermal strain-controlled low- cycle fatigue data for OFHC copper. A comparison of the predicted and experimental cyclic lives showed that an elastic analysis predicts a longer cyclic life than that observed in experiments by a factor greater than 4. The results from elastic-plastic analysis for the plate bend specimen. however. predicted a cyclic life in close agreement with experiment, thus justifying the need for the more rigorous stress-strain analysis.
One of the important life-limiting failure modes encountered by the rocket nozzle liner of the Space Shuttle Main Engine (SSME) is thermal/mechanical ratchetting of the thin (0.0635-cm) wall of copper material between the fuel/coolant channels and the hot gas wall. The ratchetting of material is toward the inside hot gas path of the rocket nozzle. When viewed in transverse (to the gas flow) cross section, the initially rectangular fueUcoolant channels tend to develop a "doghouse" shape with the roof pointed toward the centerline of the nozzle (see fig. 1 from ref. 1). This deformation mode feeds on itself and causes the thin wall to become ever thinner. The thinned area may rupture eventually and dump valu- able hydrogen fuel into the nozzle where it is burned without a significant propulsive effect. The rate of thinning (i.e.. ratchetting) has been shown analytically by Arya and Arnold (ref. 2) to be temperature. pressure, and cycle dependent. New geometric designs or new materials are required to either eliminate or drastically reduce this failure mode.
Full-scale nozzle liners are expensive to build and test for the purpose of investigating new con- figurations and construction materials. Thus, subscale liners that retain the important features of a
*NASA Resident Research Associate at Lewis Research Center.
full-scale liner have been designed, built, analyzed, and tested at the NASA Lewis Research Center (refs. 3 and 4). These too are expensive to build and test. Furthermore, the turnaround time from idea (new material, new channel configuration, fabrication, etc.) to experimental verification is unacceptably long (typically about 2 yr). Thus, if a simpler, less expensive benchmark configuration can successfully emulate the basic structural loading and failure mode of full-size hardware, tremendous savings can be achieved.
A relatively simple (ground) plate bend specimen developed at Lewis (L.J. Westfall, 1992, NASA Lewis Research Center, Cleveland, OH, private communication) is able to capture the essence of the load- ings and failure modes found in high-heat-flux, high-thermal-conductivity rocket nozzle liners such as the Space Shuttle Main Engine (SSME). The bend specimen is a flat plate with an internally pressurized single longitudinal channel that is located along the center of the plate (fig. 2). The appendix gives the manufacturing details of this specimen.
Large-displacement tests of the plate specimen were performed isothermally at a high temperature in four-point loading to simulate the large cyclic thermal strains experienced by the full-scale nozzle liner. Bending strain gradients in the plate also simulate thermal strain gradients in the nozzle liner. That this bend specimen emulates the failure mode observed in nozzle liners is seen in figure 3 where the doghouse effect is evident: the deformed configuration of the bend specimen observed in tests performed at Lewis. Therefore, we believe that this specimen meets the requirements of a less expensive benchmark configu- ration that can be used to analytically assess and experimentally verify new materials and design concepts for reducing ratchetting.
This paper analytically investigates the loading and failure modes in the surrogate bend specimen. Because the ratio of the maximum deflection of the plate to its thickness is large (greater than 0.75), small-displacement analyses for the problem produced inaccurate results. Large-displacement analyses are therefore required. Although the temperature (593 °C) of the copper plate is in its creep range, the testing frequencies are high enough (6.5 cycles/min) to justify finite-element analyses in which the time (creep) effects are neglected. The investigations reported herein were conducted by performing large- displacement finite-element analyses in conjunction with elastic and elastic-plastic constitutive models. The analytical results are displayed and discussed. The future direction of this research work is also discussed.
The geometry and dimensions of the specimen and channel are given in figure 2. Solid eight- noded brick elements with an assumed strain formulation were utilized to model the pressurized (6.2-MPa) center channel of the specimen. Because of the geometric and loading symmetry, only one- quarter of the specimen was modeled. A sensitivity study of the effect of mesh density on the results showed that a large number of elements was required for accurately capturing the high bending strain gra- dients. The presence of internal pressure in the channel, in addition to the bending gradients, necessitated the use of an even finer mesh in the channel region of the specimen. This finite-element model is shown in figure 4 and consists of 3330 elements and 4463 nodes.
Approximate Shape of Bent Specimen (Plate)
Only the maximum deflection occurring at the center of the plate was experimentally measured: hence, to determine the deflections at all other points of the plate (and its bent shape at maximum deflec- tion), an approximate elastic analysis was performed by modeling the whole plate as a solid thick plate
excluding the channel under uniform load transverse to the plate. The load was analytically increased until the calculated deflection at the center was equal to the value measured in experiments. The deflec- tions at all other points (nodes) of the plate were also recorded at this time. These displacements were later used to perform the elastic and elastic-plastic finite-element analyses by treating these latter analyses as displacement-controlled boundary value problems. All finite-element analyses were performed by using the finite-element program MARC (ref. 5). The undeformed and (calculated) deformed shapes of the solid thick plates subject to these finite-element analyses are shown in figure 5. The displacements shown are exaggerated by a factor of 5.
A one-fourth segment of the pressurized and deformed (bent) single-channel plate is shown in fig- ure 6. The undeformed configuration is presented for comparison. Displacements are exaggerated by a factor of 5 again to clearl y distinguish the two configurations. An elastic stress-strain structural analysis was performed using a finite-element discretization of this segment as described in the section Finite- Element Model. Because the problem involves large displacements of the segment in the XZ-plane, a large-displacement analysis using an updated Lagrangian formulation was adopted. The channel region of the specimen is of greatest interest; thus. only those figures that exhibit the stress and strain distributions in this region are included.
The longitudinal (X-direction) stress in the vicinity of the channel is shown in figure 7. A typical bending stress distribution is observed with tension on the upper surface, compression on the lower sur- face, and a neutral axis of zero stress in the middle. The maximum elastically calculated longitudinal stress in the channel is about 766 MPa. The stresses in the Y- and Z-directions are shown in figures 8 and 9, respectively. The Y- and Z-stresses have maximum magnitudes of about 350 and 260 MPa, respectively.
The strain distribution in the channel in the X-, Y-, and Z-directions is shown in figures 10 to 12, respectively. The maximum magnitudes of the strains occur in the X-direction (approx equal to 0.7 per- cent). Also seen in figure 10 is the X-strain, which is tensile in the top layer of the channel and compres- sive in the bottom laver. The middle of the channel has almost zero X-strain.
Elastically calculated stress values far exceed the 0.2-percent offset yield strength of OFHC cop- per (30.0 MPa) at 593 °C. Therefore, an elastic analysis of the problem is inappropriate and may lead to erroneous results. Obviously, inelastic constitutive behavior must be taken into consideration. Keeping this in mind, a large-displacement elastic and perfectly